Synthesis, Structural Characterization, and Thermal Stability of a New Layered Germanate Structure, Na4Ge16O28(OH)12
Annemieke W. C. van den Berg; Govert Baak; Hendrikus van Koningsveld; Jacobus C. Jansen; Thomas Maschmeyer; Inorganic Chemistry 43 (2004) 2888–2894; doi:10.1021/ic035272s

data_4310921
_publ_contact_author_address
;
DCT, TOCK, Julianalaan 136, 2628BL Delft, The Netherlands
;
_publ_contact_author_email       J.C.Jansen@tnw.tudelft.nl
_publ_contact_author_fax         31152784289
_publ_contact_author_name        'Jansen, J. C.'
_publ_contact_author_phone       31152786133
_publ_section_title
;
 Synthesis, Structural Characterization, and Thermal Stability of a New
 Layered Germanate Structure, Na4Ge16O28(OH)12
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              2888
_journal_page_last               2894
_journal_paper_doi               10.1021/ic035272s
_journal_volume                  43
_journal_year                    2004
_chemical_formula_sum            'Ge16 Na9.592 O40'
_chemical_formula_weight         2021.92
_space_group_IT_number           12
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_audit_creation_date             03-10-23
_audit_creation_method           Xtal3.7
_cell_angle_alpha                90.00000
_cell_angle_beta                 100.179(7)
_cell_angle_gamma                90.00000
_cell_formula_units_Z            1
_cell_length_a                   7.3216(6)
_cell_length_b                   14.3986(9)
_cell_length_c                   7.7437(6)
_cell_measurement_temperature    293
_cell_volume                     803.50(11)
_computing_data_reduction        'xtal DIFDAT ADDREF SORTRF'
_computing_molecular_graphics    xtal
_computing_publication_material  'xtal BONDLA CIFIO'
_computing_structure_refinement  'xtal CRYLSQ'
_computing_structure_solution    xtal
_diffrn_ambient_temperature      293
_diffrn_measurement_device_type  CAD4
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     .71073
_diffrn_reflns_av_R_equivalents  .021
_diffrn_reflns_av_sigmaI/netI    .05
_diffrn_reflns_limit_h_max       10
_diffrn_reflns_limit_h_min       0
_diffrn_reflns_limit_k_max       20
_diffrn_reflns_limit_k_min       0
_diffrn_reflns_limit_l_max       10
_diffrn_reflns_limit_l_min       -10
_diffrn_reflns_number            1288
_diffrn_reflns_reduction_process 'No monochr Lp applied'
_diffrn_reflns_theta_max         29.91
_diffrn_reflns_theta_min         3.16
_exptl_absorpt_coefficient_mu    14.996
_exptl_crystal_density_diffrn    4.178
_exptl_crystal_F_000             937.51
_refine_diff_density_max         4.229
_refine_diff_density_min         -3.159
_refine_ls_extinction_coef       .00000
_refine_ls_goodness_of_fit_all   5.151
_refine_ls_goodness_of_fit_ref   5.689
_refine_ls_matrix_type           full
_refine_ls_number_constraints    0
_refine_ls_number_parameters     80
_refine_ls_number_reflns         1153
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          .09
_refine_ls_R_factor_gt           .069
_refine_ls_shift/su_mean         0
_refine_ls_structure_factor_coef F
_refine_ls_weighting_scheme      sigma
_refine_ls_wR_factor_all         .078
_refine_ls_wR_factor_ref         .078
_reflns_d_resolution_high        .713
_reflns_d_resolution_low         6.436
_reflns_Friedel_coverage         0
_reflns_limit_h_max              10
_reflns_limit_h_min              -10
_reflns_limit_k_max              20
_reflns_limit_k_min              0
_reflns_limit_l_max              10
_reflns_limit_l_min              0
_reflns_number_gt                998
_reflns_number_total             1205
_reflns_threshold_expression     'F    > 2.50 sig(F   )'
_cod_data_source_file            ic035272ssi20031105_063336.cif
_cod_data_source_block           BERG1
_cod_original_sg_symbol_Hall     -c_2y
_cod_database_code               4310921